o objetivo deste estudo foi avaliar , in vitro , a qualidade do preenchimento de canais radiculares curvos com a pasta de hidrxido de clcio [ ca(oh)2 ] ultracal ( ultradent ) , associada ou no a cones de guta - percha contendo hidrxido de clcio ( calcium hydroxide plus points , roeko ) . cento e vinte razes de dentes humanos extrados , aleatoriamente distribudas em 3 faixas de curvatura ( leve - 0 a 14 ; moderada - 15 a 29 ; severa > 30 ) foram utilizadas . aps o preparo qumico - mecnico , as razes foram divididas em 4 grupos ( n=30 ) de acordo com o mtodo de aplicao da medicao intracanal : grupo 1  aplicao da pasta de ca(oh)2 com espiral de lentulo ; grupo 2  aplicao da pasta de ca(oh)2 com espiral de lentulo , seguida da introduo de um cone de ca(oh)2 ; grupo 3  aplicao da pasta de ca(oh)2 com a ponta navitip ( fornecida com o sistema ultracal ) ; grupo 4  aplicao da pasta de ca(oh)2 com a ponta navitip seguida da introduo de um cone de ca(oh)2 . as razes foram diafanizadas e avaliadas quanto  qualidade do preenchimento do tero apical dos canais por um examinador calibrado . os espcimes foram examinados em lupa estereoscpica e classificadas por escores de 1 a 4 ( desde preenchimento inadequado at preenchimento total dos canais ) . os resultados foram comparados atravs da anlise de varincia e teste post hoc de duncan com nvel de significncia de 5% . no se observaram diferenas estatisticamente significantes ( p>0.05 ) entre os graus de curvatura dos grupos 1 , 3 e 4 quanto ao preenchimento dos canais . os grupos que associaram pasta e cones de ca(oh)2 ( 2 e 4 ) apresentaram melhor preenchimento apical em relao aos demais grupos , porm essa diferena foi estatisticamente significante ( p<0,001 ) somente para as razes com curvatura severa . de acordo com os resultados deste estudo , o grau de curvatura no influenciou na qualidade do preenchimento . as tcnicas que utilizaram cones de guta percha contendo ca(oh)2 promoveram um melhor preenchimento the disinfection of the root canal system is one of the most important aspects that account for the success of endodontic therapy . the use of a calcium hydroxide [ ca(oh)2]-based intracanal dressing between sessions has a major role in decreasing the microbial population within the root canals6 . for optimal effect , ca(oh)2 should be in intimate contact with the dentinal walls , along the whole canal extension5,6,7 . nevertheless , three - dimensional filling is not easily obtained , especially in curved canals , in which failures occur mostly in the apical third4,15,17,18 . the similarity between ca(oh)2 and conventional gutta - percha points facilitates their placement into root canals up to the working length2,11,13,14 . there are no studies in the literature that associate the use of ca(oh)2 paste and points . therefore , this in vitro study evaluated the quality of ca(oh)2 paste filling , associated or not with ca(oh)2-containing gutta - percha points in curved root canals . the research project was submitted to review by research ethics committee of lutheran university of brazil and the designed methodology was approved ( process # 2004 - 138h ) . one hundred and twenty roots were selected from extracted human first molars and single - rooted teeth . buccolingual and mesiodistal radiographs were taken to confirm absence of anomalies of form and size , full development of roots and presence of a single canal per root . maxillary first molars with more than one canal in the mesiobuccal root were included in the study , but only the main canal was used . the length of the roots was standardized between 14 and 18 mm by sectioning the crowns at the cementoenamel junction . the roots were classified according to their degree of curvature as mild ( 0 to 14 ) , moderate ( 15 to 29 ) and severe ( above 30 ) , as proposed by fontanella , et al.8 ( 2004 ) . forty roots were selected for each of the three ranges of curvature degree . a size 10 k - type file was introduced into the canal until the tip of the instrument was visualized at the apical foramen . working length ( wl ) was calculated by subtracting 1 mm from this measurement . before shaping , the cervical third was prepared with sizes 1 , 2 and 3 laxxess instruments at 650 rpm . the middle and apical thirds were shaped according to the step - back technique up to a size 50 k - type file , the size 30 k - type file being the memory file . at each change of instrument , the canals were alternately irrigated with 2 ml of 1% sodium hypochlorite and 2 ml of 17% trisodium edta . , south jordan , ut , usa ) and size 30 ca(oh)2-containing gutta - percha points ( calcium hydroxide plus points ; roeko , langenau , germany ) , which were delivered to root canals following different protocols . prior to the placement of intracanal dressings , the sample received a stratified randomization to guarantee uniform distribution of the different curvature degrees in each group of treatment . group 1 : a size 25 lentulo spiral ( maillefer instruments sa , ballaigues , switzerland ) carrying small portions of ca(oh)2 paste was placed into the canals at 2 mm from the working length and powered at low speed until paste reflow was observed . petrpolis , rj , brazil ) was used at canal entrance to condense the intracanal dressing towards the root apex . group 2 : root canals were filled in the same way as described for group 1 . however , after the paste was condensed , a size 30 ca(oh)2-containing gutta - percha point was introduced into the canal up to the working length . group 3 : root canals were filled using a navitip tip ( supplied with ultracal kit ) . the navitip tip was attached to ultracal syringe and introduced into the canals up to 2 mm from the working length . the syringe embolus was then pushed and the syringe was pulled backwards slowly , until paste reflow was observed . ltda ) was used at canal entrance to condense the intracanal dressing towards the apex . group 4 : root canals were filled in the same way as described for group 3 . however , after the paste was condensed , a size 30 ca(oh)2-containing gutta - percha point was introduced into the canal up to the working length . both areas were sealed with conventional glass ionomer cement ( ketac - fill plus , espe , seefeld , germany ) , light - cured composite resin ( heraeus- kulzer , hanau , germany ) and araldite resin handled according to the manufacturers ' instructions . the teeth went through a clearing process3,10 by immersion in 5% nitric acid ( qumica delaware , porto alegre , rs , brazil ) for 72 h ( the solution being changed every 24 h ) , washing in running water for 4 h and successive dehydration in 80% alcohol for 12 h , 90% alcohol for 1 h and 99% alcohol for 3 h ( changed every hour ) . the teeth were then placed in methyl salicylate ( qumica delaware ltda . , porto alegre , rs , brazil ) , which rendered them transparent . the cleared roots were examined under a stereomicroscope ( gsz , zeiss , germany ) at 16x magnification and the quality of canal filling was assessed . a calibrated experienced examiner , blinded to curvature degrees and groups of treatment , examined all surfaces of the apical third of each root and attributed scores to the specimens according to the following ranking scale : score 1 : inadequate root canal filling  0 - 50% of intracanal space was filled ( figure 1 ) ; score 2 : root canal filling with great failures  51 - 70% of intracanal space was filled ( figure 2 ) ; score 3 : root canal filling with minor failures 71 - 85% of intracanal space was filled ( figure 3 ) ; score 4 : complete root canal filling  86 - 100% of intracanal space was filled ( figure 4 ) . intra - examiner reliability was assessed by intraclass correlation coefficient ( icc ) after reexamination of 15 specimens . data referring to the quality of filling obtained with the different techniques , as a function of curvature degree , were described as means and standard deviations . analysis of variance compared the results of the groups at curvature levels and duncan 's post hoc test identified the differences . data were assessed using spss software , version 11 ( statistical package for the social sciences , adobe systems inc . , san jose , ca , usa ) and sigma plot ( sigma - aldrich corp . during clearing procedures , 5 specimens were lost because of infiltration of liquids used in the process . means and standard deviations of the scores attributed to each group are shown table 1 . regarding the degree of curvature , it was observed that in groups 1 ( lentulo ) , 3 ( navitip ) and 4 ( navitip + point ) there were no statistically significant differences ( p>0.05 ) among the curvature ranges . in group 2 ( lentulo + point ) there was bordering statistical significance ( p=0.05 ) for severe curvature in comparison to the other curvature degrees . regarding the filling techniques , the groups that associated the use of ca(oh)2 paste and points ( 2 and 4 ) showed better filling of the apical third than the groups that received ca(oh)2 paste alone as intracanal dressing ( 1 and 3 ) . however , this difference was statistically significant ( p<0.001 ) only for the roots with severe curvature . this study evaluated the quality of intracanal dressing placement in root canals filled with ultracal ca(oh)2 paste . this paste has a new injectable application system , navitip , which was developed for use in curved canals . lentulo spirals , which are still the most indicated instruments for this purpose , were also used in comparison to the manufacturer - supplied tips4,5,12,15,17,18 . the hypothesis that the placement of ca(oh)2 points into canals filled with ca(oh)2 paste would produce an embolus effect and improve apical filling quality the roots used in this study were classified in each of the curvature ranges not only by their angulation . the initial position of curvature was also considered because both parameters determine the severity of root curvature1,11 . apical foramen was provisionally sealed with wax prior to application of intracanal dressing to prevent air escape from the canal . foramen patency could produce a falsely adequate filling that would not reflect the clinical situation18 . the findings of this study indicate that , under the investigated conditions , the quality of root canal filling was not influenced by curvature degree in the groups filled using lentulo spiral , navitip and navitip + point . there were no statistically significant differences ( p>0.05 ) among the three curvature ranges ( mild , moderate and severe ) for these groups . these results are not consistent with those of torres and luft17 ( 2003 ) , who reported better root filling quality in teeth with mild curvature than in severely curved roots , regardless of the technique used . this discrepancy of results may stem from the variability of root anatomy . far more than curvature , the complexity of the root canal systems , with its numerous ramifications , is a variable difficult to control and may either facilitate or impair the filling of the canals . bordering statistical significance ( p=0.05 ) was observed in group 2 ( lentulo + point ) when degree of curvature was compared . in this case , the action of the ca(oh)2 point seemed to be beneficial for filling severely curved canals but did not affect the quality of filling in the other curvature ranges . regarding the filling technique , groups 2 and 4 presented higher scores than the other groups in mild and moderate curvature ranges , but this difference was not significant statistically ( p>0.05 ) . the superiority of the techniques employing ca(oh)2 points was established in roots with severe curvature . in this range , groups 2 and 4 presented better root canal filling ( p<0.001 ) than the other groups in which ca(oh)2 paste alone was used . the results of this study are in agreement with those of estrela , et al.5 ( 2002 ) , who reported an adequate root canal filling when a ca(oh)2 paste prepared with an aqueous vehicle was used as an intracanal dressing . in the present study , in all groups , ca(oh)2 paste was condensed at canal entrance towards the apex using a paper point of great diameter . in the groups where ca(oh)2 points were used , condensation of the intracanal dressing occurred in apical third . these findings suggest that the physical embolus action of the ca(oh)2 point resulted in better filling quality , pushing the paste into an intimate contact with root canal walls . therefore , a similar effect may be expected if conventional gutta - percha points are used in the same way . the filling obtained with use of ultracal paste alone corroborates the findings of previous studies . this system seems to be inadequate for use in curved canals because the diameter of the tip supplied with the kit ( 0.76 mm ) is not compatible with that of severely curved root canals . according to staehle , et al.16 ( 1997 ) , needles with diameters greater than 0.6 mm can be employed only for straight canals enlarged apically at least up to a size 50 file , which did not occur in the present study . in view of these findings , it seems clear that the quality of curved root canal filling with an aqueous calcium hydroxide paste is considerably improved when ca(oh)2 points are also used . the association of paste and points seemed to make the difference , mainly in canals with more accentuated curvatures . according to the methodology proposed and based on the results of this study , the following conclusions may be drawn : 
 all techniques were unable to fill root canal apical third completely.when lentulo spiral , navitip tip and navitip + ca(oh)2 points were employed , the curvature range did not influence the quality of apical third filling.when lentulo spiral was associated with ca(oh)2 point , canals with severe curvature presented better filling than those with mild to moderate curvatures.the techniques that associated ca(oh)2 paste and point ( lentulo + point and navitip + point ) yielded better filling quality at root canal apical third in roots with severe curvature . when lentulo spiral , navitip tip and navitip + ca(oh)2 points were employed , the curvature range did not influence the quality of apical third filling . when lentulo spiral was associated with ca(oh)2 point , canals with severe curvature presented better filling than those with mild to moderate curvatures . the techniques that associated ca(oh)2 paste and point ( lentulo + point and navitip + point ) yielded better filling quality at root canal apical third in roots with severe curvature .